- Home
- Documents
*Crystallization of random copolymers ... Crystallization of Random Copolymers Isaac C. Sanchez* and*

prev

next

out of 6

View

7Download

0

Embed Size (px)

r

)

l

JOURNAL OF RESEARCH of the Notional Bureau of Standards - A. Physics and Chemistry Vol. 77A, No.3, May-June 1973

Crystallization of Random Copolymers

Isaac C. Sanchez* and R. K. Eby

Institute for Materials Research, National Bureau of Standards, Washington, D.C. 20234

(January 18, 1973)

A theory of crystallization is formulated for random copolymers which crystallize with the non- crystallizable co-units incorporated into the crystalline lattice as defects. The appropriate melting point equation and other associated thermodynamic properties are derived for this model as a function of crystal thickness and comonomer concentration. The formation of lamellar type morphology is assumed to be a kinetically determined phenomena and nucleation theory is utilized accordingly. The isothermal lamella thickness is predicted to increase in a definitive manner as the noncrystallizable comonomer concentration X increases, while the associated isothermal growth rate is predicted to decrease. The variation of lamella thickness with X when the copolymer is quenched or cooled at a uniform rate is also qualitatively predicted. Under these conditions lamella thickness decreases with increasing X, which is in accord with previous experimental observations on random copolymers of tetrafluoroethylene and hexafluoropropylene as well as other random copolymers. Theory also suggests how the surface free energy parameters (T e and (T can be d~termined from isothermal crystallization experiments for a series of random copolymers of varying composition.

Key words: Copolymers; crystallization ; growth rate; lamella thickness; melting temperature.

1. Introduction

A random copolymer can potentially crystallize in two extreme ways. It can form a two-phase system in which the crystalline phase is composed entirely of A units and is in equilibrium with a mixed amorphous phase of A units and non crystallizable comonomer B units (comonomer exclusion). Alternatively, the copolymer may form a two phase system in which the crystalline phase is a solid solution of A and B units; the comonomer B units produce defects in the crystal- line A lattice and both phases have the same composi- tion (comonomer inclusion). The question arises as to which state is more characteristic of the experi- mentally observed crystalline state. One can try to answer this question by invoking thermodynamics: if the observed state is a true thermod ynamic state, then we need only determine the state of lowest free energy. Figure 1 schematicall y illustrates the two models.

In Flory's theory of copolymer crystallization [1] I it is tacitly assumed that . the state of lowest free energy is the two phase system where the comonomer B units are excluded from the crystal. However, on a priori grounds, there is no reason to believe that the ex- clusion model is thermod ynamicall y more stable than the inclusion model. Moreover, the question as to

·Present address: Polymer Science and Engineering, University of Massachusells, Amherst , Mass. 01002. Portions of this work were carried out while an NRC-NAS Post- doctoral Research Associate at NBS.

I Figures in brackets indicate the litera ture references at the e nd of this paper.

which state is more stable is largel y academic because the observed state probably corresponds to a meta- stable state determined by kinetic factors. This is certainly the case in homopol ymer crystallization. Thick crystals are thermodynamically more stable than thin lamellar crystals with high surface to volume ratios; nevertheless, metastable lamellar morphology develops under the usual kinetic conditions of homo· polymer crystallization.

FIGURE 1. Two extreme representations of lamellar random co- polymer crystals, the exclusion model (left) and inclusion model (right).

Real copolymer crystals may exhibit a morphology intermediate to the two extremes in figure 1. In the present paper, a simple theory for random copolymer

353

crystallization is formulated which adopts the view that lamella crystalline morphology is kinetically deter- mined and that the inclusion model is more character- istic of the crystalline state. A preliminary account of this theory has been given previously [2].

In section 2 melting temperature relationships are derived as a function of copolymer composition and crystal thickness. The heats of fusion associated with the two models are also considered. In section 3 an elementary kinetic theory of crystallization is formu- lated and in section 4 the conclusions of the study are briefly outlined.

2. Thermodynamics

2.1. Equilibrium Melting Point

Melting point equations have previously been derived for the exclusion [1] and inclusion [3], [4] models. What follows is an alternative derivation of the equilibrium melting point for the inclusion model. First, we enumerate the assumptions upon which the derivation rests:

1. The heat of fusion !1H and the entropy of fusion !1S are independent of temperature; !1H(T}=!1H(T,~} and !1S(T} = !1S(T!:,} = !1H(T~)/T?n where T?n is the equilibrium melting point of the homopolymer.

2. Compositional changes do not affect the entropy of fusion; if X is the mole fraction of B co-units in the copolymers, then !1S(T, X)= !1S(T, O}= !1S(T~}.

3. The heat of fusion is a simple linear function of the number of comonomer units that enter the crystal:

!1H(T,X) = !1H(T,~) -X !1Hd (1)

where !1H d is the heat of transition (an excess enthalpy) associated with the formation of a defect in the crystal- line lattice,!1H d ;;. O.

Assumption 1 is the usual and simplest approximation employed in determining the bulk free energy differ- ence between melt and crystal; an analysis of the error inherent in this approximation has been made [5]. Assumption 2 is a good approximation if the composition of the crystal and melt are identical. Moreover, a sizable fraction of the entropy of fusion is configura- tional entropy (estimated to be about 75% for poly- ethylene [6]) which should be relatively insensitive to compositional changes. Assumption 3 is valid when comonomer defects in the crystal are isolated (low concentrations required) so that they do not interact.

When a copolymer crystal, free of nonequilibrium defects and surface effects, is in equilibrium with the melt, the melting temperature T?n is given by

(2a)

Utilization of the previously mentioned assumptions then yields

(2b)

where A == !1H dl!1H (T?n ).

2.2. Melting Temperature of Lamellar Crystals

Small crystals with high surface to volume ratios will melt at temperatures below the equilibrium melting temperature T~,. Denoting by !1G the bulk free energy difference between copolymer crystal and melt, a thin lamellar crystal of thickness l is in equilibrium with the melt when [5]

!1C - 2(J"ell = 0 (3)

where (J"e is the surface free energy of the basal plane of the lamellar crystal. For T ",; T?" the bulk free energy difference !1C(T, X) is given by

!1G(T,X) = !1H(T,X) - T!1S(T,X) (4a)

and thus from assumption 2 and eqs (I) and (2)

!1G(T,X) = !1H(T~)(T~, (X) -T) Inn' (4b)

Combining eqs (2b), (3), and (4b), the following equation for the melting temperature T mel) of a lamellar copolymer crystal obtains:

{ 2(J"e } Tm(l}= 1 - !1H (T~) Oil) - AX 1i:,. (5)

Notice that eq (5) reduces to eq (2b) for large l, as it should.

Equation (5) is slightly different in functional form than the melting point equation first derived by Eby [3], [4] for solid solution copolymer crystals. In addition to the assumptions mentioned above, there is an un- necessary series expansion; the effect of comonomer concentration and finite crystal thickness on the melt- ing temperature is evaluated to first order (higher order corrections which are small are ignored). The present derivation has avoided the use of series expan- sions and thus the melting point depression (T~ - T m) is predicted to be slightly larger by a factor T~/T m than the original Eby equation. However, ~efitting 2 the data of [4] yielded constants which agreed within the limits of error with the former ones and which did not alter the conclusions in [4].

As mentioned previously, Flory [1] assumes that the copolymer crystal is composed entirely of A units; B co-units are excluded and remain in an amorphous phase. The melting point depression is caused by the fact that preferential ordering of the copolymer chains is required for crystallization (an entropy effect) whereas in the present case, the melting point depres- sion is caused by the defective heat of fusion that accompanies the crystallization (an enthalpy effect).

J Melting point data [4] for tetrafluoroethylene and hexafluoroethylene random copolymers were reanalyzed using eq (5). The following new results were obtained: r: =612 ±4 K, CTf';= 61±23 ergs/em!, and .6.Hd=O.042±O.003 eV. , For the purposes of comparison the the original results were TUm = 617 ±S K,O'e= 77 ±27 ergs/cm 2 and 6H d = 0.047 ±O.OO3 eV.

354

'-I

For a random copolymer and low comonomer concen- trations, the Flory equation reduces to

T = (1 - A'X) TO m til (6)

where A' = RTml IlH (1~.). Comparison of eq (6) with eq (2b) shows that they are identical in form except that RTm has replaced IlHd in eq (2b) - a manifestation of the different effects considered (entropy versus en- thalpy). Although Flory did not consider the effect of crystal size on the melting temperature, such an